SEMI NAR BY Dr . KARTHI K MOHAN. I Postgraduate Student
CONTENTS Page No INTRODUCTION
MEANS OF COMPENSATION
FORMATION OF INLAY PATTERNS
Direct Wax Pattern
Indirect Wax Pattern
THE SPRUE FORMER
CASTING RING LINERS
INVESTING PROCEDURE FOR WAX PATTERNS
Hand 窶的nvesting Procedure
HEATING THE MOLD
Wax Elimination 29 CASTING MACHINES
PRACTICAL DIFFERENCES BETWEEN HYGROSCOPIC AND HIGH-HEAT TECHNICS
CAUSES OF DEFECTIVE CASTINGS
INTRODUCTION In dentistry the lost-wax casting technic was not popular unit 1907 when W.H. Taggart introduced his technic and casting machine. Today the lost-wax technic is common practice and is used for a variety of casting operations; these range form the simplest inlay to all forms of cast crowns, bridge structures, and removable partial dentures, each of which involves the same fundamental practices in forming the cast restoration.
The casting method consists of forming a wax pattern, surrounding it with investment material, and later heating the investment mold to remove the wax before casting the molten metal into the mold. Glass can be cast in a manner similar to that used with metals; thus esthetic dental crowns can be produced.
Regardless of the technic used or the type of restoration to be cast, an exact duplicate pattern of the finished restoration must first be prepared in wax or plastic. After an acceptable pattern is formed, it is surrounded with dental investment, and the investment hardens to form the mold into which the alloy is cast.
All investment materials display some setting expansion and hygroscopic expansion on hardening, and they display thermal expansion when they are heated to eliminate the wax from the mold or when they are heated to more elevated temperatures. The amount of each type of expansion varies with the technic selected and the method used to manipulate the investment. However, with any acceptable technic, the combined setting, hygroscopic, and thermal expansion should be consistent and should produce a total of 1.5% to 2% mold expansion before the casting is made.
The choice of the technic is optional,
depending on the facilities available and the operatorâ€™s preference. Each technic is influenced by variables of manipulation; therefore, to obtain reproducible and accurate results, attention must be given to all details of the procedure.
When the investment mold has been formed and the wax eliminated by heating, the mold is then ready to receive the molten metal to form the casting. Proper and careful heating of the investment mold is necessary for at least three reasons: (1) Complete wax elimination occurs only with adequate time and temperature of heating, (2)
Proper heating permits the correct thermal expansion to occur before making the casting, and
(3) Overheating of calcium sulfate â€“ bonded investment produces a chemical decomposition of the calcium sulfate.
This decomposition of the investment mold is damaging to the surface quality and physical properties of the alloys if the decomposition is excessive.
Excessive heating of the investment is especially
undesirable when embedded alloy backings, wire clasps, and other forms are included in the mold as part of the restoration. The decomposition gases within the mold embrittle the embedded alloy and prevent the formation of a good union with the cast alloy. To prevent the damaging effects of decomposition gases form calcium sulfate-bonded investment, avoid heating the investment mold to temperatures above 700Â° C and keep the heating time to the required minimum. Some calcium sulfatebonded investments contain special ingredients, such as oxalic acid and oxalate salts; on heating, such ingredients decompose and form carbon dioxide. The presence of carbon dioxide in the mold cavity depresses the decomposition of calcium sulfate.
Dimensional Changes The purpose of the dental casting is to provide a metallic replacement for missing tooth structure.
Some castings serve as a
framework to support artificial replacements of missing teeth, such as
bridges or removable partial denture restorations. A casting should be as accurate as possible, although a tolerance of + 0.05% for an inlay casting is acceptable. If the linear dimension of an average dental inlay casting is assumed to be 4mm, +0.05% of this value is equal to only +2 Âľm, which indicates that if two castings made for the same tooth have a variation of 4 Âľm, the difference may not be noticeable. To visualize this dimension, recall that the thickness of an average human hair is about 40Âľm. Therefore the tolerance limits of a dental casting are approximately onetenth of the thickness of a human hair. To obtain castings with such small tolerance limits, rigid requirements must be placed not only on the investment material but also on the impression materials, waxes, and die materials. Naturally, technical procedures and the proper handing of these materials are equally important. The absolute values for the setting, hygroscopic, and thermal expansions of investment materials may vary from one product to another, and slightly different technic may be used with different investments. In each case the values that are obtained for any one property should be reproducible form one batch to another and from one casting to another.
In general, three distinct contractions that require compensation may take place during the casting process.
1. Shrinkage of the wax pattern results form the change in the temperature at which the wax pattern is prepared and subsequently invested. The wax pattern may be prepared in the patientâ€™s mouth. 2. 2. Contraction can also result from phase changes. Recall that most materials contract during solidification.
However, when casting
alloys solidify, this contractions is minimized, and it is negligible if the wax pattern is sprued properly and an adequate casting machine during the casting operation. 2. Shrinkage of cast alloys results from the thermal coefficient of expansion. Remember that dental castings cool after solidification from the solidus temperature of the alloy to room temperature. This cooling involves contraction, the amounts of which depends on the both the alloy composition and the casting shape. For dental gold alloys, this shrinkage may vary form 1.25% to 1.7% for different alloys and castings of different shapes.
These three contractions take place in all castings, and adequate compensation is required to properly fit the restoration.
MEANS OF COMPENSATION The practical way to compensate for the shrinkage during casting is by expansion of the investment mold.
The investments currently
available exhibit three types of expansion â€“ setting, hygroscopic, and thermal.
Theoretically, the type of investment expansion that
compensates for the shrinkage is not important as long as the sum of the effective setting hygroscopic, and thermal expansions is sufficient to compensate for all the shrinkages. The dimensional changes that occur in the casting operation are summarized at the end of this section.
The various techniques used in casting operations can be classified into two main groups: (1) The high-heat or thermal expansion technic and (2) The low-heat or hygroscopic technic. If the majority of the compensation for shrinkages is produced by the thermal expansion of the investment, and the technic is described as a high-heat, or thermal expansion, technic. Conversely, if the majority of the compensation for the shrinkage is accomplished by investment is known as a hygroscopic type of investment and the technic is described as a low-heat, or hygroscopic, technic.
Alloy Shrinkage =
FORMATION OF INLAY PATTERNS The factors of flow, expansion, warpage, and others are all important in preparing an inlay wax pattern that will produce an accurate gold casting.
Regardless of the procedure followed, the physical
principles that govern the basic nature of the wax also control the behavior of the pattern during and following formation. The method of preparing a wax pattern is called direct if the wax pattern is prepared in the patientâ€™s mouth.
Conversely, if an impression of the cavity
preparation is taken and a die is formed from the impression on which the pattern is prepared, the method is called indirect.
Direct Wax Patterns Type I wax for a direct wax pattern must be heated sufficiently to have adequate flow and plasticity under compression to reproduce all details of the cavity walls. Adequate compression of the wax is required in forming direct wax patterns. Also, overheating of the wax should be avoided because of possible tissue damage and discomfort to the patients, as well as the difficulty encountered in compression of the very fluid overheated wax.
When the wax is heated to the proper working temperature of approximately 50째C to 52째C for a short period, the previously induced stress form manufacturing and handling tends to be dissipated. A stressfree piece of wax at the proper consistency should be obtained so that the pattern, when formed under pressure, remains relatively stress-free. Thus minimal distortion results when the pattern is subsequently removed form the tooth. This heating and annealing of the wax before insertion into the cavity preparation is accomplished most easily and effectively in a small dry-heat oven. A non-uniform consistency and possible volatilization of some of the wax mass tends to result from excessively heating the wax over a Bunsen burner flame. Prolonged heating of the wax in water, especially at high temperatures, may result in a crumbly mass. Although wax may be annealed in water that is at a proper temperature, it should not be stored for long periods under these conditions.
Because wax has rather low thermal conductivity, cooling form the working temperature to mouth temperature occurs slowly, and ample time for cooling should be allowed. The decrease in temperature of the wax to mouth temperature results in a contraction. This contraction is offset to some degree when the pattern is held under pressure until mouth temperature is reached because the compression stresses tend to be released, to some degree, when the wax is removed form the prepared
tooth. However, the degree and distribution of these stresses vary from one pattern to another. Although these induced stresses are undesirable, their presence is unavoidable.
Because carving a wax pattern directly in the mouth is a task demanding a high degree of dexterity, any property that eases manipulation is desirable. Therefore ANSI/ADA Specification No.4 for wax states that the wax should be of a color that contracts with the hard and soft tissues of the mouth; the wax should often without becoming flaky; and the wax should not show appreciable chipping or flaking when trimmed to a fine margin.
Carving instruments that have been
sufficiently warmed are desirable to that have been sufficiently warmed are desirable to soften, but not melt, the wax as the marginal adaptation and contour are developed. The warm instrument brings the portion of the wax that its proper working temperature, so that less stress is induced in these areas. A cool carving instrument burnishing over or cutting through the wax introduces both tension and compression stresses into the pattern, which are detrimental to the ultimate fit of the casting.
Indirect Wax Patterns When a wax pattern is formed by the indirect method, a metal or stone die is used, which is the positive replica of at least a portion of the
surrounding tooth structure and the cavity preparation. This tooth replica permits the pattern to be formed outside of the mouth. Forming the wax pattern on a die permits a change in the type of wax and certain manipulative procedures that are necessary for the direct inlay technic. The convenience provided by the indirect method makes the property of flow less critical, because the pattern may be removed form the die at a lower temperature and with greater ease.
When adapting wax to stone or some metal dies, some form of lubricant must be used to release the wax patter from the die. In the mouth no such lubricant is required because a thin film of saliva or dentinal fluid serves as a lubricant. A variety of fluids are currently available to prevent the attachment of the wax to the die. These fluids produce a separator film of minimum thickness. An excess of separator is to be avoided because it leads to inaccuracies in the wax pattern and poor surface of the cast alloy.
The wax may be adapted to the die either by the flowing of small melted increment from a spatula to build up the desired contour or by the compression method, as is suggested in the direct technic methods. By either method the temperature of a stone die is of little concern in wax adaptation, because the stone is a poor thermal conductor. Likewise, the
temperature of a metal die is not critical when compression of the wax is used to form the pattern. However, this temperature is critical when molten increments are used to build up the pattern because the manner of solidification of the wax depends on the temperature of the metal die.
When molten wax flows onto a cool metal die, the wax immediately adjacent to the die solidifies rapidly because the heat form the molten wax is rapidly dissipated. The wax adjacent to the air stays molten for a longer period, and as it solidifies and contracts, it pulls the previously congealed wax away form the metal, resulting in poor surface adaptation.
Conversely, if the metal die is warmed throughout to near body temperature, the wax solidifies more evenly throughout its mass, resulting in better adaptation.
The die can be warmed by placing it under an electric lamp or placing it with the carving instruments on an electric heating pad that is at a suitable temperature. The indirect wax pattern is carved with a warm instrument, as is the direct pattern, again to minimize the formation of stresses in the wax.
Because of the basic physical nature of the wax, distortion of the pattern is a continual hazard. Not only does wax have one of the highest coefficients of thermal expansion of any dental material, but it also possess a relatively low softening temperatures that may cause stress release or flow to occur. Stresses are easily induced in forming any pattern; in fact, the formation of a completely stress-free wax pattern would appear improbable.
With knowledge of the physical
characteristics of the inlay wax, the operator must minimize the stress within the pattern by applying manipulative procedures that permit proper temperature and stress control of the wax.
THE SPRUE FORMER The purpose of a sprue former, or sprue pin, is to provide a channel through which molten alloy can reach the mold in an invested ring after the wax has been eliminated. With large restorations or prostheses, such as removable partial denture frameworks and fixed partial dentures, the sprue formers are made of wax.
The diameter and length of the sprue former depend to a large extent on the type and size of the pattern, the type of casting machine to be used, and the dimensions of the flask or ring in which the casting is to
be made. Prefabricated sprue formers are available in a wide range of gauges or diameters.
Sprue former gauge selection is often empirical, yet it is based on the following five general principles: Select the gauge sprue former with a diameter that is approximately the same size as the thickest area of the wax pattern. If the pattern is small, the sprue former must also be small because a large sprue former attached to a thin, delicate pattern could cause distortion. However, it the sprue former diameter is too small, this area will solidify before the casting itself and localized shrinkage porosity (“suck-back” porosity) may develop. Reservoir sprues are used to help overcome this problem. If possible, the sprue former should be attached to the portion of the pattern with the largest cross-sectional areas. It is best for the molten alloy to flow form a thick section to surrounding thin areas (e.g., margins) and not the reverse. This design minimizes the risk for turbulence. Also, the sprue former orientation should minimize the risk of metal flow onto flat areas of the investment or small areas such as line angles.
Gauge No. B & S 6 8 10 12 14 16 18
Diameter Cm 0.4115 0.3264 0.2588 0.2053 0.1628 0.1291 1.1024
Inches 0.1620 0.1285 0.1019 0.08081 0.06408 0.05082 0.04030
Wax patterns sprued directly (left and right). On the right is an example of indirect spruing showing a reservoir bar that is positioned near the heat center of the invested ring. ď ś The length of the sprue former should be long enough to properly position the pattern in the casting ring within 6 mm of the trailing end and yet short enough so the molten alloy does not solidify before it fills the mold. ď ś The type of sprue former selected influences the burnout technique used.
Wax sprue formers are more common than plastic.
advisable to use a two-stage ensure complete carbon elimination, because plastic sprues soften at temperatures above the melting point of inlay waxes.
ď ś Patterns may be sprued either directly or indirectly.
spruing, the sprue former provides a direct connection between the pattern area and the sprue base or crucible former area. With indirect spruing, a connector or reservoir bar is positioned between the pattern and the crucible former. It is common to use indirect spruing for multiple single units and fixed partial dentures, although several single units can be sprued with multiple direct sprue formers.
A reservoir should be added to a spruing network to prevent localized shrinkage porosity. When the molten alloy fills the heated casting ring, the pattern area should solidify first and the reservoir last. Because of its large mass of alloy and position in the heat center of the ring, the reservoir remains molten of furnish liquid alloy into the mold as it solidifies. The resulting soldification shrinkage occurs in the reservoir bar and not in the restorations, assuming that the reservoir bar is larger in volume than that of the patterns and that the sprue formers attached to those patterns were placed in the appropriate position and were of the correct gauge.
Sprue Former Attachment. The sprue former connection to the wax pattern is generally flared for higher density gold alloys but is often restricted for lower density alloys. Flaring of the sprue former may act in
much the same way as a reservoir, facilitating the entry of the fluid alloy into the pattern area.
Sprue Former Position.
The position of the sprue former
attachment is often a matter of individual judgment, based on the shape and form of the wax pattern. Some clinicians prefer placement at the occlusal surface, whereas others choose sites such as a proximal wall or just below a nonfunctional cusp to minimize subsequent grinding of occlusal anatomy and contact areas. As indicated earlier, the ideal area for the sprue former is the point of greatest bulk in the pattern and to permit a smooth flow3 of the alloy.
Sprue Former Direction. The sprue former should be directed away from any thin or delicate parts of the pattern, because the molten metal may abrade or fracture investment in this area and result in a casting failure. It should not be attached at a right angle to a broad flat surface. Such an orientation of the sprue former leads to turbulence within the mold cavity and severe porosity in this region. When this same pattern is sprued at a 45-degree angle to the proximal area, a satisfactory casting is obtained.
Sprue Former Length. The length of the sprue former depends on the length of the casting ring. If the sprue is toot short, the wax pattern may be so far removed form the end of the casting ring that gases cannot be adequately vented to permit the molten alloy to fill the ring completely. When these gases are not completely eliminated, porosity may result. Therefore, the sprue length should be adjusted so that the top of the wax pattern is within 6 mm of the open end of the ring for gypsumbonded investments.
With the higher-strength phosphate-boned
investments, it may be possible to position it within 3 to 4 mm of the top of the investment. For reproducibility of casting accuracy, the pattern should be placed as close to the center of the ring as possible.
Wax Pattern Removal. The sprue former should be attached to the wax pattern with the pattern on the master die, provided the pattern can be removed directly in line with its path of withdrawal form the die. Any motion that might distort the wax pattern should be avoided during removal.
CASTING RING LINERS With the use of solid metal rings or casting flasks, provision must be made to permit investment expansion. The mold may actually become smaller rather than larger because of the reverse pressure resulting from
the confinement of the setting expansion. This effect can be overcome by suing a split ring or flexible rubber ring that permits the setting expansion of the investment.
However, the most commonly used technique to provide investment expansion is to line the walls of the ring with a ring liner. Traditionally, asbestos was the material of choice, but it can no longer be used because its carcinogenic potential makes it a biohazard. Two types of non-asbestos ring liner materials have been produced: an aluminum silicate ceramic liner and a cellulose (paper) liner.
To ensure uniform expansion, the liner is cut to fit the inside diameter of the casting ring with no overlap. The dry liner is tacked in position with sticky wax and then is use either dry or wet. With a wet liner technique, the lined ring is immersed in water for a time, and the excess water is shaken away. Squeezing the liner should be avoided because this leads to variable amounts of water removal and uneven expansion. Although a ceramic liner may to absorb water like a cellulose liner, its network of fibers can retain water on the surface.
Not only does the liner afford greater normal setting expansion in the investment, but also the absorbed water causes a semi-hygroscopic expansion as it is drawn into the investment during setting. The use of
one liner increases the normal setting expansion compared with no liner. A thicker liner material or two layers of liner provide even greater semihygroscopic expansion and also afford a more unrestricted normal setting expansion of the investment. As shown in the figure, two layers of liner can be used to increase the expansion slightly compared with that obtained form one liner. In any case, the thickness of the liner should not be less than approximately 1 mm.
Cellulose liners, being paper products are burned away during the burnout procedure, so a technique must be found to secure the investment in the ring. However, the desired length of the liner remains a matter of controversy. If the length of the liner is somewhat shorter that the ring itself, the investment is confined at one or both ends of the ring. The longitudinal setting and hygroscopic expansion are there by restricted, as compared with an end where the liner is flush with the ends of the ring.
The expansion of the investment is always greater in the unrestricted longitudinal direction than in the lateral direction, that is, toward the ring itself. Therefore, it is desirable to reduce the expansion in the longitudinal direction. Placing the liner somewhat short of the ends of ht erring tends to produce a more uniform expansion; thus, there is less chance for distortion of the wax pattern and the mold.
INVESTING PROCEDURE FOR WAX PATTERNS After the wax pattern for an inlay or other small restoration, such as a crown or bridge abutment, has been prepared and sprued, and a surface tension-reducing agent has been applied, it then should be invested promptly. The correct water powder ratio of the investment mix, a required number of spatulation turns, and a proper investing technic are essential to obtain acceptable casting results. There are tow different methods of investing the wax pattern: hand investing and vacuum investing.
Hand 窶的nvesting Procedure The recommended water/powder ratio always should be followed for best results.
Usually 50 g of calcium sulfate-bonded investment
powder or 60g of phosphate-bonded investment powder is sufficient to fill an inlay ring. A correct amount of water or special liquid is measured and placed in a rubber mixing bowl, and then the investment powder is added. The powder and liquid are mixed briefly with a plaster spatula until all the powder is wetted. The cover of the bowl, which carries the mechanical mixer, is placed over the bowl, and the mix is spatulated. The mixing bowl and a hand mechanical spatula.
Mixing bowl and hand mechanical spatula.
While spatulating, the manufacturerâ€™s recommendations should be followed carefully; usually 100 turns of the spatulator are adequate.
With the hygroscopic investment, the setting of an investment depends critically on the number of spatulation turns, which affects the hygroscopic expansion.
The investment, after being spatulated, is placed on the vibrator to eliminate some of the air bubbles form the mix and to collect all of the mix form the sides of the rubber bowl into the center. A sprue base with sprue, wax pattern, and ring.
Sprue base, sprue pin with wax pattern, and ceramic paper lined casting ring.
The sprue base, which holds the sprue and wax pattern, is held with one hand, ad the investment is painted over the wax pattern with a camelhair brush. In painting the pattern, the investment should be teased ahead of the brush to prevent incorporation of air adjacent to the pattern. After the painting is completed, the pattern is vibrated very gently with the spruie base held firmly with the fingers and the under side of the hand resting on the vibrator. This method relieves any minor air bubbles that might have been trapped around the wax pattern. Then the inlay ring is placed over the sprue base and filled.
For the setting and hygroscopic expansion of an investment to take place more uniformly, some allowance must be made for the lateral
expansion of the investment. Solid rings do into permit the investment to expand laterally during the setting, hygroscopic, and thermal expansions of the mold. To over come this lateral restriction, a ceramic paper liner is placed inside the ring, and liner in position.
Assembled sprue base and metal casting ring. The ceramic paper liner is cut to fit the inside of the metal ring and is held in place wit the fingers. The ring containing the liner is then dipped into water until the liner is completely wet and water is dripping form it. The ring is shaken gently to remove the excess water. Variable amounts of water in the liner produce different amounts of hygroscopic expansion in the investment, regardless of the type of investment used. After the liner has been soaked, it should not be touched or adapted further with the fingers because this reduces its cushioning effect, which is needed for the lateral expansion of the investment. A liner that is about
3 mm short at each end of the ring is preferred. When the liner is equally short at each end of the ring, the investment is locked into the ring, and uniform expansion of the cavity form occurs.
After the pattern has been painted with investment, the liner is properly adapted, and the ring is properly assembled on the sprue base, the mixed investment is poured into the ring, which is held at a slight angle so that the investment flows slowly down its side to fill form the bottom to the top. In this manner the possibility of trapping quantities of air in the ring, or around the pattern, is reduced to a minimum.
It is often helpful to hold the assembled ring and sprue base in one hand, which rests gently on a vibrator while the investment is being poured into the ring. When the ring is completely filled, it is leveled with the top by the edge of a plaster spatula. The filled ring is then set aside for the investment to set completely filled, it is leveled with the top by the edge of a plaster spatula.
The filled ring is then set aside for the
investment to set completely, which usually requires 45 to 60 minutes.
When a phosphate investment is used the ring is slightly overfilled, the top of the ring is not leveled off, and the investment is allowed to set. After the investment has set, the excess investment is ground off using a
model trimmer. This procedure is necessary because a nonporous, glassy surface results, which must be ground off in order to improve the permeability of the investment and allow for gases the readily escape from the mold during the casting step.
Vacuum-Investing Procedure Vacuum-investing equipment is available to facilitate the investing operation. A popular vacuum machine that is used in dentistry. With this equipment the powder and water, or special liquid, are mixed under vacuum, and the mixed investment is permitted to flow into the ring and around the wax pattern wit the vacuum present.
investing does not remove all the air from the investment and the inlay ring, the amount of air usually is reduced enough to obtain a smooth adaptation of the investment to the pattern. Vacuum investing often yields castings with improved surfaces when compared with castings produced from hand-invested patterns. The degree of difference between the two procedures depends largely on the care used in hand investing.
Whether hand-or vacuum-investing procedures are used in filling the casting ring, the investment should be allowed to harden in air if the thermal expansion technic is used. Conversely, if the hygroscopic waterimmersion technic is used. The casting ring containing the investment
should be placed immediately in a water bath at 37째C, and the investment should be allowed to harden under water.
An inlay-casting ring
containing a ceramic paper liner and investment after setting using the water bath immersion technic is ready for burnout of the wax.
One type of vacuum unit for investing small wax pattern
Investment mold ready for burnout.
Investing Patterns for Water-Added Technic The hand-and vacuum-investing procedures apply to any technic and can be practiced regardless of whether a high-heat or hygroscopic casting technic is used. However, certain technics may require some minor changes to accommodate the particular method. For example with the water-added hygroscopic technic, in which a controlled amount of water is added to the investment in the ring to provide the desired hygroscopic expansion of the investment, a regular metal ring with ceramic paper liner cannot be used.
In the water-added technic a flexible rubber ring capable of expanding laterally without any liner is used. A set of commercially available equipment for the water-added technic.
Equipment needed for water-added hygroscopic expansion technic.
And it consists of a flexible sprue base, a flexible ring that fits the sprue base, a metallic sleeve to facilitate the handing of the flexible ring, a reservoir to provide extra room for water to be added after the wax pattern is invested and the metallic sleeve removed, and a hypodermic syringe to accurately deliver a prescribed amount of water. With this equipment the wax pattern can be invested by either a hand-investing or a vacuum-investing technic, as described previously.
HEATING THE MOLD After the wax pattern has been invested, it should be set aside until the investment mass is hardened. A requirement in all investments is to wait until the final set of the investment before placing it in an oven for elimination of the wax pattern. Usually 45 to 60 minutes are required after the start of the mix for the investment to reach its final set and to possess a sufficiently high wet strength to be transferred to the oven.
The strength of the investment is an important property of an investment in any technic, especially with the water-added technic, in which a flexible rubber ring is used instead of a metallic rig a ceramic liner. With regular technic the metallic ring containing the investment and the wax pattern is placed in the oven for wax elimination. After the wax has been eliminated and the mold has reached the casting temperature, the molten metal is cast into the mold cavity while the mold is supported by the metallic ring.
In this way the mold can better
withstand the impact force exerted by the molten metal entering the hot mold.
With water-added techniques, the water reservoir, flexible
ring, sprue, and base are removed, and a cylinder of the investment without a supporting ring is placed in the sprue.
Mold with invested wax pattern ready for removal of the sprue and heating for wax elimination After the wax is eliminated, the molten metal is forced into the investment without support of a metal ring. Therefore, the investment used with this technic should not only have a high strength, but also should have adequate time (at least 45 minutes) to reach its maximum wet strength before being placed into the oven.
Wax Elimination The mold is placed in an oven to completely eliminate the wax, thereby forming a cavity into which the molten metal is cast. During wax elimination the investment expands thermally, which is necessary to compensate for to casting shrinkages.
Although wax melts at a
comparatively low temperature, its complete elimination requires much higher temperatures. Usually, if elimination is not complete, small bits of
the wax residue are retained in the fine margins of the mold and prevent the formation of a complete casting. When the molten metal enters the sprue hole, the resulting force causes the air in the mold cavity to be driven out through the pores of the investment, and thus the mold cavity is filled completely. The presence of any foreign material in the mold cavity slows down or possibly prevents the air or other gases form being driven out of the mold before the molten metal solidifies. As a result, the castings are incomplete or the margins are irregular, in which case casting should be repeated, starting with a new wax pattern.
Because the ingredients of inlay waxes are organic materials, they are composed of carbon, hydrogen, and nitrogen. When heated to higher temperatures, any organic materials decompose and forms carbon dioxide (CO2), water (H2O), or nitrogen oxide (NO), all of which are gaseous and can be easily eliminated. However, formation of these gases depends on the presence of a sufficient of the oven, and adequate heating time of the ring. If the amount of oxygen available to the wax in the mold cavity is not sufficient, the temperature of the oven is not high enough, or the wax pattern is heated only for a short time, incomplete reaction between the wax and oxygen may result.
A satisfactory way of eliminating the wax pattern is to set the mold in the furnace with the sprue hole placed downward at first, so that most of the wax drains out and is eliminated as a liquid. The ring is then inverted with the sprue hole placed upward. In this position the oxygen in the oven atmosphere can wax, and form gases rather into the cavity, react with the wax, and form gases rather than the fine carbon that interferes with the venting of the mold cavity. The lower the mold temperature and the larger the wax pattern, the longer the mold should be left in the oven. For a 500째 C mold temperature and larger wax patterns, the mold should remain in the oven for approximately 1 hour, with the sprue hole placed downward during half of this time and upward during the other half. If more than one ring is placed in an oven, a longer period is required for wax elimination. The general rule is to add 5 minutes to the wax elimination time for every extra ring placed in the oven at 500째C. with an oven temperature of 600째 to 700째C, a shorter time may be sufficient to completely eliminate the wax..
Oven Temperature Investment materials are poor heat conductors, which results in some temperature difference between the inner core and the outside portion of the mold. Although this difference is relatively great at the beginning of the heating cycle, it diminishes the time progresses and may
cease to exist at the time of casting. The difference in temperature between the inner and outer portions of the mold becomes greater if the mold is placed in a preheated oven or if the heating rate of the oven is too rapid. The outside of the mold, being exposed to a higher temperature, expands somewhat more than does the inner part. This expansion may cause the mold to crack during the heating period. Because of the high thermal expansion of investment s containing cristobalite, the difference in the temperatures of different portions of the mold may create uneven expansion. For best results this type of investment should always be placed in a room-temperature oven, with the oven temperature increased slowly. The difference in the temperature of different portions of the mold does not affect quartz-containing investments, probably because the rate of thermal expansion of the quartz investment is slower than that of the cristobalite investment. With hygroscopic investments, in which the thermal expansion of the investment is only about 0.5%, the mold can be placed in a preheated oven of 500째C and not crack during the heating.
When the wax pattern is completely eliminated and the mold has reached the casting temperature, the alloy is melted by an appropriate method and cast into the mold cavity.
CASTING MACHINES Alloys are melted in one of three following ways, depending on the available types of casting machines: The alloy is melted in a separate crucible by a torch flame and the metal is cast into the mold by centrifugal force The alloy is melted electrically by a resistance or induction furnace, then cast into the mold centrifugally by motor or spring action. Representative casting machines of these types are shown in Figures 23-9 and 23-10, respectively. The alloy is melted as in the first two ways, but it is cast by air pressure, a vacuum, or both.
The general procedure for each is described in the following sections, with certain advantages and disadvantages cited. However, it is important to follow the manufacture’s directions precisely.
Centrifugal Casting Machine. The casting spring is first wound from tow to five turns (depending on the particular machine and the speed of casting rotation desired). The metal is melted by a torch flame in a glazed ceramic crucible attached to the “broken arm” of the casting machine. The broken-arm feature accelerates the initial rotational speed of the crucible and casting ring, thus increasing the linear speed of the
liquid casting alloy as it moves into and through the mold. Once the metal has reached the casting temperature and the heated casting ring is in position, the machine is released and the spring triggers the rotational motion.
As the metal fills th4e mold there is a hydrostatic pressure gradient develops along the length of the casting. The pressure gradient from the tip of the casting to the bottom surface is quite sharp and parabolic in form, reaching zero at the button surface.
Ordinarily, the pressure
gradient at the moment before solidification begins reaches about 0.21 to 0.28 MPa (30 to 40psi) at the tip of the casting. Because of this pressure gradient, there is also a gradient in the heat transfer rate such that the greatest rate of heat transfer to the mold is at the high pressure end of the gradient (i.e., the tip of the casting). Because this end also is frequently the sharp edge of the margin of a crown, there is further assurance that the solidification progresses from the thin margin edge to the button surface.
Centrifugal casting machine, spring wound
Casting machine, spring wound, electrical resistance, melting furnace
Electrical Resistance-heated Casting Machine. In this instance there is an automatic melting of the metal in a graphite crucible within a furnace rather than by use of a torch flame.
This is an advantage,
especially for alloys such as those used for metal-ceramic restorations, which are alloyed with base metals in trace amounts that tend to oxidize on overheating. Another advantage is that the crucible in the furnace is located flush against the casting ring.
Therefore, the metal button
remains molten slightly longer, again ensuring that solildification progresses completely from the tip of the casting to the button surface. A
carbon crucible should not be used in the melting of high palladium or palladium-silver alloys, where the temperature exceeds 1504째C or with nickel-thromium or cobalt-thromium base metal alloys. An example of the electrical resistance casting machine.
Induction Melting Machine. With this unit, the metal is melted by an induction field that develops within a crucible surrounded by watercooled metal tubing. Once the metal reaches the casting temperature, it is forced into the mold by air pressure, vacuum, or both, at the other end of the ring. The device has become popular in the casting or jewelry but has not been used as much as the other tow techniques for noble alloy castings. It is more commonly used for melting base metal alloys.
There is little practical difference in the properties or accuracy of castings made with any of the three types of casting machines. The choice is a matter of access and personal preference.
Casting Crucibles. Generally, three types of casting crucibles are available: clay, carbon, and quartz (including zircon-alumina).
crucibles are appropriate for many of the crown and bridge alloys, such as the high noble types. Carbon crucibles can be used not only for high
noble crown and bridge alloys but also for the higher-fusing, gold-based metal ceramic alloys.
Quartz crucibles are recommended for high-fusing alloys of any type. They are especially suited for alloys that have a high melting range and are sensitive to carbon contamination. Crown and bridge alloys with a high palladium content, such as palladium-silver alloys for metalceramic copings, and any of the nickel-based or cobalt-based alloys are included in this category.
PRACTICAL DIFFERENCES BETWEEN HYGROSCOPIC AND HIGH-HEAT TECHNICS In the hygroscopic technic the setting and hygroscopic expansions of the investment are major factors in compensating for the shrinkage of the cast alloy and wax pattern.
The thermal expansion of such
investments is rather low. In the high-heat technic the thermal expansion of the investment compensates mainly for the shrinkage, and the setting and hygroscopic expansion of such investments are rather low. The net expansion should be the same with either type of investment. When heating the investment to obtain thermal expansion of the investment, the wax pattern melts and the mold cavity can expand without any interference from the wax pattern.
However, during setting and
hygroscopic expansion of the investment, the wax pattern is present and offers some resistance to the expansion forces. For example, the setting and hygroscopic expansions of the investment inside the core for the full crown type of pattern are restricted by the strength of the wax pattern. A bulkier pattern offers more resistance than the normal-sized wax pattern. Similarly, full crowns made of hard inlay wax offer more resistance than those made of regular or soft wax. However, note that the type of wax used for making one-surface inlays has very little effect. In this instance the investment expands away from the wax patstern, and the strength of the wax cannot alter the expansion. In all other cases, the type of the wax used with the hygroscopic technic is important in the fit of the resulting castings.
In general, regular or soft waxes should be used with the
hygroscopic technic. The use of hard inlay wax or a plastic pattern in the hygroscopic technic is even greater than with the water bath immersion technic the temperature of the pattern because of its thermal expansion. In the water-added technic the invested wax pattern remains near room, temperature, and neither its rigidity nor its dimensions are altered.
Cleaning the Casting. Let us first consider the gold crown and bridge alloys. After the casting has been completed, the ring is removed and quenched in water as soon as the button exhibits a dull-red glow. Two advantages are gained in quenching: (1) the noble metal alloy is left
in a n annealed condition for burnishing, polishing, and similar procedures, and (2) when the water contacts the hot investment, a violent reaction ensues. The investment becomes soft and granular, and the casting is more easily cleaned.
Often the surface of the casting appears dark with oxides and tarnish. Such a surface film can be removed by a process known as pickling, which consists of heating the discolored casting in an acid. Probably the best pickling solution for gypsum-bonded investments is a 50% hydrochloric acid solution.
The hydrochloric acid aids in the
removal of any residual investment as well as of the oxide coating. The disadvantage of the use of hydrochloric acid is that the fumes form the acid are likely to corrode laboratory metal furnishings. In addition, these fumers are a health hazard and should be vented via a fume hood. A solution of sulfuric acid is more advantageous in this respect. Ultrasonic devices are also available for cleaning the casting, as are commercial pickling solutions made of acid salts.
The best method for pickling is to place the casting in a test tube or dish and to pour the acid over it. It may be necessary to heat the acid, but boiling should be avoided because of the considerable amount of acid fumes involved. After pickling, the acid is poured off and the casting is
removed. The pickling solution should be renewed frequently because it is likely to become contaminated with use.
In no case should the casting be held with steel tongs so that both the casting and the tongs come into contact with the pickling solution, as this may contaminate the casting. The pickling solution usually contains small amounts of copper dissolved form previous castings. When the steel thongs contact this electrolyte, a small galvanic cell is created and copper is deposited on the casting at the point where the tongs grip it. This copper deposition extends into the metal and is a future source for discoloration in the area.
It is a common practice to heat the casting and then to drop it into the pickling solution. The disadvantage of this method is that a delicate margin may be melted in the flame or the casting may be distorted by the sudden thermal shock when plunged into the acid.
Gold-based and palladium-based metal-ceramic alloys and base metal alloys are bench cooled to room temperature before the casting is removed form the investment. Castings from these alloys are generally not pickled, and when it is recommended for certain metal-ceramic alloys, it is only to selectively remove specific surface oxides.
CAUSES OF DEFECTIVE CASTINGS An unsuccessful casting results in considerable trouble and loss of time. In almost all instances, defects in casting can be avoided by strict observance of procedures governed by certain fundamental rules and principles. Seldom is a defect in a casting attributable to other factors than the carelessness or ignorance of the operator.
techniques, casting failures should be the exception, not the rule.
Defects in castings can be classified under four headings: (1) Distortion (2) Surface roughness and irregularities (3) Porosity (4) Incomplete or missing detail. Some of these factors have been discussed in connection with certain phases of the casting techniques.
The subject is summarized and
analyzed in some detail in the following sections.
Any marked distortion of the casting is probably
related to a distortion of the wax pattern, as described in the chapter on inlay wax. This type of distortion can be minimized or prevented to proper manipulation of the wax and handling of the pattern.
Unquestionably, some distortion of the wax pattern occurs as the investment hardens around it. The setting and hygroscopic expansions of the investment may produce an uneven movement of the walls of the pattern.
This type of distortion occurs in part from the uneven outward movement of the proximal walls. The gingival margins are forced apart by the mold expansion, whereas the solid occlusal bar of wax resists expansion during the early stages of setting. The configuration of the pattern, the type of wax, and the thickness influence the distortion that occurs, as has been discussed. For example, distortion increases as the thickness of the pattern decreases. As would be expected, the less the setting expansion of the investment, the les is the distortion. Generally, it is not a serious problem expect that it accounts for some of the unexplained inaccuracies that may occur in small castings.
probably not a great deal that can be done to control this phenomenon.
Surface Roughness, Irregularities, and Discoloration.
surface of a dental casting should be an accurate reproduction of the surface of the wax pattern from which it is made. Excessive roughness or irregularities on the outer surface of the casting necessitate additional
finishing and polishing, whereas irregularities surface prevent a proper seating of an otherwise accurate casting.
Surface roughness should not be confused with surface irregularities. Surface roughness is defined as relatively finely spaced surface imperfections whose height, width, and direction establish the predominant surface pattern.
Surface irregularities refer to isolated
imperfections, such as nodules, that do not characterize the total surface area.
Even under optimal conditions, the surface roughness of the dental casting is invariably somewhat greater than that of the wax pattern form, which it is made. The difference is probably related to the particle size of the investment and its ability to reproduce the wax pattern in microscopic detail.
With proper manipulative techniques, the normal increased
roughness in the casting should not be a major factor in dimensional accuracy. However, improper technique can lead to a marked increase in surface roughness, as well as to the formation of surface irregularities.
Air Bubbles. Small nodules on a casting are caused by air bubbles that become attached to the pattern during or subsequent to the investing procedure. Such nodules can sometimes be removed if they are not in a
critical area. However, for nodules on margins or on internal surfaces, removal of these irregularities might alter the fit of the casting. As previously noted, the best method to avoid air bubbles is to use the vacuum investing technique.
If a manual method is used, various precautions can be observed to eliminate air form the investment mix before the investing.
previously outlined, the use of a mechanical mixer with vibration both before and after mixing should be practiced routinely. A wetting agent may be helpful in preventing the collection of air bubbles on the surface of the pattern, but it is by no means a certain remedy. As previously discussed, it is important that the wetting agent be applied in a thin layer. It is best to air dry the wetting agent, because any excess liquid dilutes the investment, possibly producing surface irregularities on the casting.
Water Films. Wax is repellent to water, and if the investment becomes separated from the wax pattern in some manner, a water film may form irregularly over the surface. Occasionally, this type of surface irregularity appears as minute ridges or veins on the surface.
If the pattern is moved slightly, jarred, or vibrated after investing, or if the painting procedure does not result in an intimate contact of the
investment with the pattern, such a condition may result. A wetting agent is of aid in the prevention of such irregularities. Too high an L:P ratio may also produce these surface irregularities.
Rapid Heating Rates. This factor has been discussed in a previous section. It results in fins or spines on the casting similar to those, or a characteristic surface roughness may be evident because of flaking of the investment when the water or steam pours into the mold. Furthermore, such a surge of steam or water may carry some of the salts used as modifiers into the mold, which are left as deposits on the walls after the water evaporates. As previously mentioned, the mold should be heated gradually; at least 60 minutes should elapse during the heating of the investment-filled ring from room temperature to 700째C. The greater the bulk of the investment, the more slowly it should be heated.
Under heating. Incomplete elimination of wax residues may occur if the heating time is too short or if insufficient air is available in the furnace.
These factors are particularly important with the low-
temperature investment techniques. Voids or porosity may occur in the casting from the gases formed when the hot alloy comes in contact with the carbonaceous residues. Occasionally, the casting may be covered
with a tenacious carbon coating that is virtually impossible to remove by pickling.
Liquid: Powder Ratio.
The amount of water and investment
should be measured accurately. The higher the L:P ratio the rougher the casting. However, if too little water is used, the investment may be unmanageably thick and cannot be properly applied to the pattern. In vacuum investing, the air may not be sufficiently removed. In either instance, a rough surface on the casting may result.
Prolonged Heating. When the high-heat casting technique is used, a prolonged heating of the mold at the casting temperature is likely to cause a disintegration of the investment, and the walls of the mold are roughened as a result. Further more, the products of decomposition are sulfur compounds that may contaminate the alloy to the extent that the surface texture is affected. Such contamination may be the reason that the surface of the casting sometimes does not respond to prickling. When the thermal expansion technique is employed, the mold should be heated to the casting temperature â€“never higher than 700Â°C and the casting should be made immediately.
Temperature of the Alloy. If an alloy is heated to too high a temperature before casting, the surface of the investment is likely to be attacked, and a surface roughness of the type described in the previous section may result. As previously noted, in all probability the alloy will not be overheated with a gas-air torch when used with the gas supplied in most localities. If other fuel is used, special care should be observed that the color emitted by the molten gold alloy, for example, is no lighter than a light orange.
Casting Pressure. Too high a pressure during casting can produce a rough surface on the casting. A gauge pressure of 0.10 to 0.14 MPa in an air pressure casting machine or three to four turns of the spring in an average type of centrifugal casting machine is sufficient for small castings.
Composition of the Investment. The ratio of the binder to the quartz influences the surface texture of the casting. In addition, a coarse silica causes a surface roughness.
If the investment meets ADA
Specification No.2, the composition is probably not a factor in the surface roughness.
Foreign Bodies. When foreign substance gets into the mold, a surface roughness may be produced.
For example, a rough crucible
former wit investment clinging to it may roughen the investment on its removal so that bits of investment are carried into the mold with the molten alloy. Carelessness in the removal of the sprue former may be a similar cause.
Usually, contamination results not only in surface roughness but also in incomplete areas or surface voids. An example may be see at C in any casting that shows sharp, well-defined deficiencies indicates the presence of some foreign particles in the mold, such as pieces of investment and bits of carbon form a flux. Bright-appearing concavities may be the result of flux being carried into the mold with the metal.
Surface discoloration and roughness can result from sulfur contamination,
temperatures or from a high sulfur content of the torch flame.
interaction of the molten alloy with sulfur produces black castings that are brittle and do not clean readily during pickling.
Impact of Molten Alloy. The direction of the sprue former should be such that the molten gold alloy does into strike a weak potion of the
mold surface. Occasionally, the molten alloy may fracture or abrade the mold surface on impact, regardless of its bulk. It is unfortunate that sometimes the abraded area is smooth so that it cannot be detected on the surface of the casting. Such a depression in the mold is reflected as a raised area on the casting, often too slight to be noticed yet sufficiently large to prevent the seating of the casting. This type of surface roughness or irregularity can be avoided by proper spruing so as to prevent the direct impact of the molten metal at an angle of 90 degrees to the investment surface. A glancing impact is likely to be less damaging, and at the same time an undesirable turbulence is avoided.
Pattern Position. If several patterns are invested in the same ring they should not be placed too close together.
Likewise, too many
patterns positioned in the same plane in the mold should be avoided. The expansion of wax is much greater than that of the investment, causing breakdown or cracking of the investment if the spacing between patterns is less that 3 mm.
Carbon Inclusions. An improperly adjusted torch, or a carboncontaining investment, can be absorbed by the alloy during casting. These particles may lead to the formation of carbides or even create visible carbon inclusions.
There are certain surface discolorations and
roughness that may not be evident when the casting is completed but that may appear during service. For example, various gold alloys, such as solders, bits of wire, and mixtures of different casting alloys should never be melted together and reused. The resulting mixture would not possess the proper physical properties and might form eutectic or similar alloys with low corrosion resistance. Discoloration and corrosion may also occur.
A source of discoloration often overlooked is the surface contamination of a gold alloy restoration by mercury. Mercury penetrates rapidly into the alloy and causes a marked loss in ductility and a greater susceptibility to corrosion. Thus, it is not a good practice to place a new amalgam restoration adjacent to high noble alloy restoration. In addition, these dissimilar metals form a galvanic cell that can lead to breakdown of the anode (amalgam) relative to the cathode (noble alloy).
Porosity. Porosity may occur both within the interior region of a casting and on the external surface. The latter is a factor in surface roughness, but also it is generally a manifestation of internal porosity. Not only does the internal porosity weaken the casting but if it also extends to the surface, it may be a cause for discoloration. If severe, it
can produce leakage at the tooth-restoration interface, and secondary caries may result. Although the porosity in a casting cannot be prevented entirely, it can be minimized by use of proper techniques. Porosities in noble metal alloy castings may be classified as follows: I.
Solidification defects A. Localized shrinkage porosity B. Microporosity
Trapped gases A. Pinhole porosity B. Gas inclusions C. Subsurface porosity
Localized shrinkage is generally caused by incomplete feeding of molten metal during solidification. The linear contraction of noble metal alloys in changing from a liquid to a solid is at least 1.25%. therefore, there must be continual feeding of molten metal through the sprue to make up for the shrinkage of metal volume during solidification. If the sprue freezes in its cross section before this feeding is completed to the casting proper, a localized shrinkage void will occur in the last portion of the casting that solidifies. Four types of porosity are
(a) Localized shrinkage porosity; (b) Micros porosity; (c) Pinhole porosity; and (d) Subsurface porosity.
Localized shrinkage generally occurs near the sprue-casting junction, but it may occur anywhere between dendrites, as shown in where the last part of the casting that solidified was in the low melting metal that remained as the dendrite branches develop.
This type of void may also occur externally, usually in the interior of a crown near the area of the sprue, if a hot spot has been created by the hot metal impinging from the sprue channel on a point of the mold wall. This hot spot causes the local region to freeze last and result in what is called suck-back porosity, as shown. This often occurs at an occlusoaxial line angle or incisoaxial line angle that is not well rounded. The entering metal impinges onto the mold surface at this point and creates a higher localized mold temperature in this region that is called a hot spot. A hot spot may retain a localized pool of molten metal alter other areas of the casting have solidified. This in turn creates a shrinkage void, or suckback porosity. Such-back porosity can be eliminated by flaring the point
of sprue attachment an by reducing the mold-melt temperature differential, that is, lowering the casting temperature by about 30째C.
Microporosity also occurs from solidification shrinkage but is generally present in fine grain alloy castings when the solidification is too rapid for the microvoids to segregate to the liquid pool. This premature solidification is too rapid for the microvoids to segregate to the liquid pool. This premature solidification causes the porosity shown in and portions of the form of small irregular voids.
Such phenomena can occur form the rapid solidification if the mold or casting temperature is too low. It is unfortunate that this type of defect is not detectable unless the casting is sectioned. In any case, it is generally not a serious defect. The effects of various factors involved in formation of microporosity, and other types of porosity, are summarized.
Both the pinhole and the gas inclusion porosities are related to the entrapment of gas during solidification. Both are characterized by a spherical contour, but they are decidedly different in size.
inclusion porosities are usually much larger than pinhole porosity, as indicated in. Many metals dissolve or occlude gases while they are molten. For example, both copper and silver dissolve oxygen in large
amounts in the liquid state. Molten platinum and palladium have a strong affinity for hydrogen as well as oxygen. On solidification, the absorbed gases are expelled and the pinhole porosity results. The larger voids may also result from the same cause, but it seems more logical to assume that such voids may be caused by gas that is mechanically trapped by the molten metal in the mold or that is incorporated during the casting procedure. All castings probably contain a certain amount of porosity, exemplified by the photomicrographs shown in. However, the porosity should be kept to a minimum because it may adversely affect the physical properties of the casting.
Oxygen is dissolved by some of the metals, such as silver, in the alloy while they are in the molten state. During solidification, the gas is expelled to form blebs and pores in the metal. As was pointed out earlier, this type of porosity may be attributed to abuse of the metal. Castings that are severely contaminated with gases are usually black when they are removed from the investment and do into clean easily on pickling. The porosity that extends to the surface is usually in the form of small pinpoint holes when the surface is polished, other pinholes appear.
Larger spherical porosities can be caused by gas occluded from a poorly adjusted torch flame, or the use of the mixing or oxidizing zones
of the flame rather than the reducing zone. These types of porosity can be minimized by pre-melting the gold alloy on a graphite crucible or a graphite block if the alloy has been used before and by correctly adjusting and positioning the torch flame during melting.
Subsurface porosity occurs on occasion as is shown in and at other times it may be particularly evident. The reasons for such voids have not been completely established. They may be caused by the simultaneous nucleation of solid grains and gas bubbles at the first moment that the metal freezes at the mold walls. As has been explained, this type of porosity an be diminished by controlling the rate at which the molten metal enters the mold.
Entrapped air porosity on the inner surface of the casting, sometimes referred to back-pressure porosity, can produce large concave depressions such as those seen. This is caused by the inability of the air in the mold to escape through the pores in the investment or by the pressure gradient that displaces the air pocket toward the end of the investment via the molten sprue and button. The entrapment is frequently found in a â€œpocketâ€? at the cavity surface of a crown or mesio-occlusal casting. Occasionally, it is found even on the outside surface of the casting when the casting temperature or mold is so low that solidification
occurs before the entrapped air can escape. The incidence of entrapped air can be increased by the dense modern investments, an increase in mold density produced by vacuum investing, and the tendency for the mold to clog with residual carbon when the low-heat technique is used. Each of these factors tends to slow down the venting of gases form the mold during casting.
Proper burnout, an adequate mold and casting temperature, a sufficiently high casting pressure, and proper L:P ratio can help to eliminate this phenomenon. It is good practice to make sure that the thickness of investment between the tip of the pattern and the end of the ring not be greater than 6 mm.
Occasionally, only a partially completely
casting, or perhaps no casting at all, is found. The obvious cause is that the molten alloy has been prevented, in some manner, form completely filling the mold. At least two factors that might inhibit the ingress of the liquefied metal are insufficient venting of the mold and high viscosity of the fused metal.
The first consideration, insufficient venting, is directly related to the backpressure exerted by the air in the mold. If the air cannot be
vented quickly, the molten alloy does not fill the mold before if solidifies. In such a case, the magnitude of the casting pressure should be suspected. If insufficient casting pressure is employed, the backpressure cannot be overcome. Furthermore, the pressure should be applied for at least 4 seconds. The mold is filled and the metal is solidified in 1 second or less, yet it is quite soft during the early stages. Therefore, the pressure should be maintained for a few seconds beyond this pint.
Examples of an
incomplete casting because of insufficient casting pressure are shown. These failures are usually exemplified in rounded, incomplete margins.
A second common cause for an incomplete casting is incomplete elimination of wax residues from the mold. If too many products of combustion remain in the mold, the pores in the investment may become filled so that the air cannot be vented completely. If moisture or particles of wax remain, the contact of the molten alloy with these foreign substances produces an explosion that may produce sufficient back pressure to prevent the mold form being filled. All example of a casting failure caused by incomplete wax elimination can be seen in although similar to the incomplete casting in it can be noted that the rounded margins are quite shiny rater than dull. This shiny condition of the metal is caused by the strong reducing atmosphere created by carbon monoxide left by the residual wax.
The possible influence of the L:P ratio of the investment has already been discussed. A lower L:P ratio is associated with less porosity of the investment. An increase in casting pressure during casting solves this problem.
Different alloy compositions probably exhibit varying viscosities in the molten state, depending on composition and temperature. However, both the surface tension and the viscosity of a molten alloy are decreased with an increase in temperature. An incomplete casting resulting form too great a viscosity of the casting metal can be attributed to insufficient heating. The temperature of the alloy should be raised higher than its liquidus temperature so that its viscosity and surface tension are lowered and it does not solidify prematurely as it enters the mold. Such premature solidification may account for the greater susceptibility of the white gold alloys to porosity because their liquidus temperatures are higher. Thus, they are more difficult to melt with a gas-air torch flame.
1. M.A.MARZOUK, A.L.SIMONTON, R.D.GROSS. “Operative Dentistry” Ishiyaku EuroAmerica, Inc, 1997: 373-386.
2. CLIFFORD M.STURDEVANT. “The art and science of Operative Dentistry”, Mosby, 3rd Edn, 1997: 688-773.
3. VIMAL K SIKRI. “Textbook of Operative Dentistry”, CBS Publishers: 269-287.
4. A. PARAMESHWARAN, K. S. KARTHIKEYAN. “Materials in Restorative Dentistry”, Meenakshiammal Trust, 1998: 91-105.
5. ROBERT CRAIG. “Restorative Dental Materials”, Mosby, 10th Edn, 1997: 437-466.
6. KENNETH J. ANNUSAVICE. “Philip’s Science of dental materials”, W. B. Saunders Company, 10th Edn, 1996: 491-524.
The Indian Dental Academy is the Leader in continuing dental education , training dentists in all aspects of dentistry and offering a wide r...